HAL Id: hal-01576312
https://hal.archives-ouvertes.fr/hal-01576312Submitted on 25 Sep 2020
HAL is a multi-disciplinary open access archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
metal/oxide interfaces and applications
B. Dieny, M. Chshiev
To cite this version:
B. Dieny, M. Chshiev. Perpendicular magnetic anisotropy at transition metal/oxide interfaces and applications. Reviews of Modern Physics, American Physical Society, 2017, 89 (2), pp.025008. �10.1103/RevModPhys.89.025008�. �hal-01576312�
Perpendicular magnetic anisotropy at transition metal/oxide
interfaces and applications
B. Dieny*and M. Chshiev†
Univ. Grenoble Alpes, INAC-SPINTEC, F-38000 Grenoble, France, CEA, INAC-SPINTEC, F-38000 Grenoble, France,
and CNRS, SPINTEC, F-38000 Grenoble, France (published 28 June 2017)
Spin electronics is a rapidly expanding field stimulated by a strong synergy between breakthrough basic research discoveries and industrial applications in the fields of magnetic recording, magnetic field sensors, nonvolatile memories [magnetic random access memories (MRAM) and especially spin-transfer-torque MRAM (STT-MRAM)]. In addition to the discovery of several physical phenomena (giant magnetoresistance, tunnel magnetoresistance, spin-transfer torque, spin-orbit torque, spin Hall effect, spin Seebeck effect, etc.), outstanding progress has been made on the growth and nanopatterning of magnetic multilayered films and nanostructures in which these phenomena are observed. Magnetic anisotropy is usually observed in materials that have large spin-orbit interactions. However, in 2002 perpendicular magnetic anisotropy (PMA) was discovered to exist at magnetic metal/oxide interfaces [for instance CoðFeÞ=alumina]. Surprisingly, this PMA is observed in systems where spin-orbit interactions are quite weak, but its amplitude is remarkably large—comparable to that measured at Co=Pt interfaces, a reference for large interfacial anisotropy (anisotropy ∼1.4 erg=cm2¼ 1.4 mJ=m2). Actually, this PMA was found to be very common at magnetic metal/oxide interfaces since it has been observed with a large variety of amorphous or crystalline oxides, including AlOx, MgO, TaOx, HfOx, etc. This PMA is thought to be the result of electronic hybridization between the oxygen and the magnetic transition metal orbit across the interface, a hypothesis supported by ab initio calculations. Interest in this phenomenon was sparked in 2010 when it was demonstrated that the PMA at magnetic transition metal/oxide interfaces could be used to build out-of-plane magnetized magnetic tunnel junctions for STT-MRAM cells. In these systems, the PMA at the CoFeB=MgO interface can be used to simultaneously obtain good memory retention, thanks to the large PMA amplitude, and a low write current, thanks to a relatively weak Gilbert damping. These two requirements for memories tend to be difficult to reconcile since they rely on the same spin-orbit coupling. PMA-based approaches have now become ubiquitous in the designs for perpendicular STT-MRAM, and major microelectronics companies are actively working on their development with the first goal of addressing embedded FLASH and static random access memory-type of applications. Scalability of STT-MRAM devices based on this interfacial PMA is expected to soon exceed the 20-nm nodes. Several very active new fields of research also rely on interfacial PMA at magnetic metal/oxide interfaces, including spin-orbit torques associated with Rashba or spin Hall effects, record high speed domain wall propagation in buffer/magnetic metal/oxide-based magnetic wires, and voltage-based control of anisotropy. This review deals with PMA at magnetic metal/oxide interfaces from its discovery, by examining the diversity of systems in which it has been observed and the physicochemical methods through which the key roles played by the electronic hybridization at the metal/oxide interface were elucidated. The physical origins of the phenomenon are also covered and how these are supported by ab initio calculations is dealt with. Finally, some examples of applications of this interfacial PMA in STT-MRAM are listed along with the various emerging research topics taking advantage of this PMA.
I. Introduction 2
II. PMA at Magnetic Transition Metal/Oxide Interfaces:
A Historical Perspective 5
A. First observation with AlOx formed by rf oxidation
and natural oxidation 5
B. A general phenomenon at magnetic metal/oxide
C. Correlation between PMA and electron-specular
reflection in specular spin valves 7 D. Physicochemical characterization (XAS, XPS) of the
metal/oxide interface and correlation with anisotropy 7
E. Influence of annealing 10
F. Correlation between PMA and tunnel magnetoresistance
in MgO-based MTJ 11
G. First observations of PMA at Ta=CoFeB=MgO
H. Interfacial PMA in epitaxial Fe=MgO-based systems 14 I. Gilbert damping measurements in
CoFeB=MgO-based MTJ 14
III. Physical Origin of the Interfacial PMA 15 A. Qualitative description of anisotropy based
on electronic hybridization 16
B. Ab initio calculations, comparison with
experimental data 18
IV. STT-MRAM Based on Interfacial CoFeB=MgO PMA 23
A. STT-MRAM: A subclass of MRAM 23
B. In-plane magnetized STT-MRAM with reduced
demagnetizing field 24
C. Perpendicular STT-MRAM 26
D. Benefit of exploiting the interfacial PMA at CoFeB=MgO interfaces when tackling the large
anisotropy or low critical current dilemma 26 E. Influence of various parameters on the PMA measured
at CoFeB=MgO interfaces 27
1. Influence of buffer and capping layers 27 2. Influence of the presence of Mg between MgO and
3. Influence of CoFeB composition on PMA amplitude
and thermal variation 28
4. Influence of annealing 30
a. Controlling the diffusion of atomic species 30 b. Influence of irradiation with light ions 31
F. Status of STT-MRAM development 32
V. Voltage Control of the Anisotropy and Applications
in Low-power Magnetic Memories 34
VI. Other Emerging Phenomena in Structures Based on Magnetic
Metal/Oxide Interfacial PMA 40
VII. Conclusion 45
VIII. Acronyms 45
The properties of magnetic thin films and multilayers first triggered interest more than 60 years ago (Néel, 1954). Since then, a wealth of new phenomena have been discovered in these artificially made material systems. These phenomena are of interest not only from a fundamental point of view but also because they could have applications in various areas including, but not limited to, magnetic storage [hard disk drives (HDD) (Thompson and Best, 2000; Chappert, Fert, and Van Dau, 2007)], solid-state magnetic memories [magnetic random access memories (MRAM) (Huai, 2008;Khvalkovskiy et al., 2013)], hybrid complementary metal oxide semiconductor (CMOS) or magnetic logic (Dieny et al., 2010; Kawahara, 2011), rf components (Rippard et al., 2005; Dussaux et al., 2010; Choi et al., 2014; Miwa et al., 2014), magnetic field sensors (Reig, Cardoso de Freitas, and Mukhopadhyay, 2014), and biotechnology (Tartaj et al., 2005). All this research and development (R&D) was made possible thanks to the tremen-dous technological progress achieved in techniques for depo-sition of magnetic thin films, in tools for their nanopatterning, in structural and chemical characterization techniques, and in the means to measure their physical properties. Among the remark-able phenomena and devices discovered and developed over the years, the following are of particular interest: the phenomenon
of exchange bias at ferromagnetic/antiferromagnetic interfaces (Meiklejohn, 1962;Nogues and Schuller, 1999); the observa-tion of perpendicular magnetic anisotropy (PMA) in thin films and enhanced magneto-optical Kerr rotation (Carcia, Meinhaldt, and Suna, 1985; Den Broeder et al., 1987; Den Broeder, Hoving, and Bloemen, 1991); giant magnetoresistance (GMR) (Baibich et al., 1988;Binasch et al., 1989), for which A. Fert and P. Grünberg were awarded the 2007 Physics Nobel Prize; low-field GMR spin valves (Dieny et al., 1991), which were made commercially available in HDD by IBM in 1998; the oscillatory exchangelike coupling between ferromagnetic (FM) layers separated by a nonmagnetic layer (Parkin, More, and Roche, 1990); tunnel magnetoresistance (TMR) at room tem-perature (Miyazaki and Tezuka, 1995;Moodera et al., 1995); the fact that it should be possible to manipulate the magneti-zation of magnetic nanostructures by spin-transfer torque (Berger, 1996; Slonczewski, 1996), and its first applications in excitation of spin waves (Tsoi et al., 1998) or magnetization switching (Wegrowe et al., 1999; Katine et al., 2000); the prediction and observation of giant tunnel magnetoresistance in MgO-based crystalline magnetic tunnel junctions (MTJ) (Butler et al., 2001;Mathon and Umerski, 2001;Parkin et al., 2004; Yuasa et al., 2004); the strong interplay between charge-spin-heat currents was harnessed and gave rise to the field of spin caloritronics (Saitoh et al., 2006;Bauer, Saitoh, and Van Wees, 2012); the prediction that spin angular momentum can be transferred from the lattice to the local magnetization by a current flow resulting in spin-orbit torques (SOT) (Manchon and Zhang, 2009); and the first observations of SOT-induced magnetization switching due to Rashba or spin Hall effects (SHE) (Miron et al., 2010;Miron, Garello et al., 2011;Liu, Lee et al., 2012;Liu, Pai et al., 2012).
Since their introduction in 1954, the development of magnetic HDD has been a strong driving force in micromagnetism, nanomagnetism, and spin electronics. The HDD industry has followed a road map very similar to the well-known Moore’s law in the semiconductor industry, where the number of components per unit area doubles every two years (i.e., 41% increase per year). Thus in HDDs, the areal density of information stored has increased at an average rate of 60% per year, representing more than 8 orders of magnitude over 50 years.
Information can be stored very efficiently by controlling the orientation of small magnetic domains (bits). For binary storage, the magnetic media onto which information is written is designed to have two stable states at remanence. This is achieved with uniaxial magnetic anisotropy, which provides a preferred orientation for the magnetization. The magnetization therefore has two possible directions along the anisotropy axis. This uniaxial anisotropy is generally characterized by an anisotropy energy per unit volume Ku, so that the anisotropy
energy varies depending on the orientation of the magneti-zation ⃗M with respect to the easy axis of magnetimagneti-zation (ˆn unit vector along this axis) as
E¼ −KuðM ⇀
To allow the increase in areal density in granular HDD media consisting of CoCrPt alloy grains, the size had to be steadily decreased as the storage density increased.
At today’s densities, around 700 Gbit=in2, the grain size is approximately 7 nm. The number of grains per bit has also decreased over time, from more than 100 initially to about 10 nowadays. Writing the information requires the magnetization of the grains to switch from one stable state to the other by overcoming an energy barrier ΔE, which separates the two stable states. The energy required is given by
ΔE ¼ KuV; ð2Þ
where Kuis the anisotropy per unit volume of the storage layer
and V its volume, i.e., the grain size. ΔE determines the stability of the written information. If the barrier is not high enough, the magnetization of a grain may accidently switch to the opposite direction due to thermal fluctuations (kBT). This
will result in degradation of the information stored. The typical time for switching by overcoming the energy barrier is given by an Arrhenius law
τ ¼ τ0exp ΔE kBT ; ð3Þ
whereτ0 is a characteristic attempt time of the order of 1 ns. For the information to remain stable throughout a specified retention time tretention(typically 10 years in HDD), the energy
barrier must comply with ΔE > kBT log tretention τ0 ; ð4Þ i.e., ΔE ¼ KuV >45kBT ð5Þ
for a 10-year retention. Over the years, as the storage density increased, the volume of grains had to be decreased. Therefore, to fulfill the condition KuV >45kBT, the
anisotropy had to be increased correspondingly. This was achieved by improving the texture of the hcp-CoCr-based alloys, reinforcing the spin-orbit coupling by Pt doping and, most importantly, by switching from in-plane to out-of-plane anisotropy to reduce the negative impact that demagnetizing energy has on the effective anisotropy as the bit size decreased (Piramanayagama, 2007). Today, the areal density in HDD is close to 1 Tbit=in2, but conventional recording technology, based on perpendicular media and classical write heads, is approaching the limit associated with the writability of the media. Indeed, the anisotropy of the media has been increased so much to fulfill the magnetic stability criterion that the field produced by the write head, which is determined by the magnetization of the head pole piece, is no longer sufficient to overcome the KuV barrier to switch
magnetiza-tion. To circumvent this issue, new approaches are being developed using graded media (Suess et al., 2005) or using recordings assisted either by microwaves [microwave-assisted magnetic recording (MAMR) (Zhu, Zhu, and Tang, 2008)] or by temporarily heating the media using a plasmonic antenna [heat assisted magnetic recording (HAMR) (Stipe et al., 2010)].
Magnetism can also be used to store data in solid-state memories, known as MRAM. These memories, unlike HDD, have no moving parts. In 1995 TMR was observed in MTJ at room temperature (RT) (Miyazaki and Tezuka, 1995;Moodera et al., 1995), and subsequently it was proposed that MTJs could serve as memory elements. An MTJ consists of two magnetic layers separated by an insulating tunnel barrier. The resistance of the barrier depends on the relative orientation of the magnetization in the two magnetic layers. In a parallel magnetic configuration, electrons can easily tunnel through the barrier, therefore the MTJ is in a low resistance state. With antiparallel alignment, electron tunneling is hampered, producing a high resistance state in the MTJ. MTJs are usually designed so that one of the two magnetic layers, the reference layer, has a fixed magnetization. The magnetization of the second layer, the storage layer, can be modified either by pulses of magnetic field or by using the spin-transfer-torque (STT) phenomenon. For further details, see Dieny et al. (2010) and Sec. IV. In MRAM, memory retention is once again directly related to the barrier height KuV. As in magnetic recording, if the memory
cell size is reduced to increase the storage capacity, the anisotropy also has to be increased to meet the criterion for thermal stability. This stability is measured for MRAM based on the failure rate in standby. For an N-bit memory, the failure rate can be calculated as a function of time by writing the probability that at least one failure will occur during a period t as 1 minus the probability that no such failure will occur in any of the N bits during the same period. This yields the following expression: FðtÞ ¼ 1 − expð−Nt=τÞ ¼ 1− exp −Nt τ0 exp −kΔE BT : ð6Þ
For a given retention time t¼ tretention and a given chip
capacity, this relationship sets a minimum value for the thermal stability ratioΔE=kBT and therefore for KuV.
These considerations show that the anisotropy of a mag-netic material plays a key role in important applications of magnetism, particularly those related to memory and storage. Magnetic anisotropy in thin films and multilayers has been studied for more than 60 years (Néel, 1954). It is now known that magnetic anisotropy can have bulk and interfacial con-tributions stemming from a common origin: the spin-orbit interaction (SOI). This interaction links the orbital motion of the electrons, which is determined by the lattice arrangement, to their spin, which constitutes the main contribution to magnetization in magnetic transition metals. Therefore the spin-orbit interaction induces pairing between the magneti-zation and the crystallographic lattice (Bethe, 1929;Bloch and Gentile, 1931; Ballhausen, 1962; Mattheiss, 1972). This interaction is associated with a number of important phenom-ena in magnetism such as magnetic anisotropy, the relaxation of magnetic excited states toward the lattice, as characterized by Gilbert dampingα, or magnetostriction phenomena. Large anisotropies are commonly observed in materials which have large spin-orbit interactions, such as heavy elements (Pt, Au, Ta, W, Bi, rare earths with nonzero orbital momentum, etc.). Indeed, conventionally the spin-orbit-coupling constant in the simplest model of atom description with Bohr radius scales as Z4. More precisely, the spin-orbit-coupling energy is
proportional toα2 Z4, whereα is the fine structure constant. However, for d elements this is oversimplified and overesti-mated since it neglects screening effects due to the outer electrons. More detailed theoretical investigations indicate that the spin-orbit-coupling energy may scale as α2 Z2, in particular, in transition metals (Khomski, 2014).
Characteristic examples of multilayers considered to have large anisotropy associated with a large spin orbit are Co=Pd and Co=Pt multilayers (Johnson et al., 1995). In bulk form, examples of systems with large anisotropy include hexagonal CoPtCr alloys which are used in media for HDD and FePt L10 -ordered alloys with tetragonal distortion (Gehanno et al., 1997). In these two examples, the reduced crystal symmetry combined with the large spin orbit of Pt results in strong magnetocrystalline anisotropy (MCA). In multilayers, the anisotropy can be of various origins. As early as 1954, Néel (1954) proposed a pair model according to which the broken symmetry at interfaces can generate anisotropy. Another contribution can arise from the crystallographic mismatch between neighboring elements generating strains in the layers which produces anisotropy due to magnetostric-tion effects (Johnson et al., 1995). Electron hybridizamagnetostric-tion across the interface may also increase the levels of degeneracy between orbitals, generating interfacial anisotropy (Daalderop, Kelly, and Schuurmans, 1994a,1994b).
In addition to these contributions, which are related to the material itself, for magnetostatic reasons the shape of the magnetic element also contributes to the anisotropy measured. In infinite thin films, in the absence of other forms of anisotropy, magnetization will spontaneously lie in the plane of the film (easy-plane anisotropy). Energy
where Msis the spontaneous magnetization in SI units, must
be supplied to bring it out of plane. If the film is patterned in small elements, the precise demagnetizing coefficients corre-sponding to the sample geometry must be taken into account (Beleggia et al., 2005). For a thin magnetic film placed between two interfaces, the anisotropy is usually expressed as an effective anisotropy per unit volume, thus,
Keff ¼ Kv−μ0 2M2s þKs t ; ð8Þ
where Kv accounts for all the material bulk anisotropy
con-tributions, −ðμ0=2ÞM2s represents the demagnetizing energy,
and Kscombines all the interfacial contributions from the two
interfaces. Experimentally, the product Kefft can be plotted
against t to determine the various contributions. The slope of this curve gives the net bulk anisotropy, whereas the intercept with vertical axis yields the net interfacial anisotropy.
This review deals with a particular form of interfacial perpendicular anisotropy (iPMA) which was discovered to exist at the interface between magnetic transition metals and oxides (Monso et al., 2002). iPMA was subsequently observed with a large variety of amorphous and crystalline oxides as well as with various transition metals such as Co, Fe, and CoFe or CoFeB alloys (Rodmacq et al., 2003, 2009; Manchon et al., 2008; Nistor et al., 2009). This is a
remarkable phenomenon considering that the amplitude of the anisotropy measured is on the scale of that found at Co=Pt interfaces (∼1.4 erg=cm2¼ 1.4 mJ=m2) even though all the elements involved (Co, Fe, Al, Mg, O, etc.) are rather light and therefore have weak spin-orbit interactions. Detailed physico-chemical characterizations [x-ray absorption (XAS) and x-ray photoemission (XPS)] revealed that this interfacial anisotropy was produced by the formation of chemical bonds between the oxygen ions of the oxide and the ions of the adjacent transition metal (Manchon et al., 2008;Rodmacq et al., 2009). Ab initio calculations later confirmed that hybridization between the sp-oxygen orbitals and the dz2orbitals in the transition metal (Co or Fe) and the ensuing decrease in degeneracy in the transition metal d orbitals cause this anisotropy (Yang et al., 2011).Ikeda et al. (2010)reported that this anisotropy could be used to prepare MgO-based out-of-plane magnetized tunnel junctions for spin-transfer-torque magnetic random access memories (STT-MRAM) exhibiting large TMR thanks to good crystallinity combined with low critical current for switching by STT thanks to a low Gilbert damping. These observations triggered considerable interest. Indeed, in the context of STT-MRAM development, out-of-plane magnet-ized MTJs have been shown to offer much better scale-down capacity than their in-plane counterparts. Indeed, the PMA can be much larger than in-plane anisotropy (IMA) in sputtered films. In-plane anisotropy in sputtered films of practical interest for MRAM is due to shape anisotropy provided by giving the MRAM cell an elongated shape but this yields a typical anisotropy field in the 100–200Oe. In contrast, PMA can yield an effective anisotropy field of several kOe. This capacity explains why today most R&D efforts devoted to MRAM focus on these out-of-plane magnetized MTJs combining high anisotropy and low damping. Major micro-electronics companies are now actively working on the development of STT-MRAM which is expected to be scalable to, and beyond, the 16-nm node.
This phenomenon of iPMA at magnetic transition metal/ oxide interfaces is therefore of great interest not only from a basic research point of view, but also for applications, in particular, magnetic memories.
Several other research areas have recently emerged that take advantage of this iPMA, and they have become active research topics. One example is voltage control of magnetism in metallic systems (Weisheit et al., 2007;Shiota et al., 2012), which could pave the way toward very low-power nonvolatile memories and logic devices. Along these lines, the iPMA at magnetic metal/ oxide interfaces was found to be tunable by applying a voltage across the oxide layer (Schellekens et al., 2012;Shiota et al., 2009). Even though the magnetic layer is metallic, the electrical field can penetrate the magnetic layer to a depth corresponding to the Thomas-Fermi screening length, to induce effects on the electronic density of states (DOS) around the interface. Since iPMA is interfacial in origin, this effect is large enough to yield a significant variation in iPMA as a function of the bias voltage. This creates a unique way to manipulate the magnetic properties in thin films by applying voltage rather than current, and, in particular, a new means to switch magnetization through the use of voltage pulses in memory devices (Shiota et al., 2012).
In contrast to out-of-plane magnetized Co=Pt-based multi-layers, films based on CoðFeÞ=oxide interfaces were observed to exhibit much lower magnetization pinning. Thus, despite their very large out-of-plane anisotropy, their coercivity, a few Oe, is much weaker than that of (Co=Pt) multilayers of several kOe. This low coercivity makes them interesting for studies of domain wall (DW) propagation in out-of-plane magnetized systems. Indeed, record domain wall speeds were obtained in this type of system (Miron et al., 2011; Schellekens et al., 2012), and they could therefore be good candidates for racetrack memories (Parkin, Hayashi, and Thomas, 2008).
In addition, the intrinsic electrical field which exists at the magnetic metal/oxide interface (Ibrahim et al., 2016b) due to charge transfer between the metal and the oxygen atoms in the oxide produces an interfacial Rashba effect. This effect can be harnessed to switch the magnetization of the magnetic metallic layer or to generate steady state magnetic excitations with an in-plane current in three-terminal magnetic tunnel junctions (Miron, Garello et al., 2011). Both Rashba and SHE (Liu, Pai et al., 2012) yield SOT which can be used to design three-terminal devices with the potential to become ultrafast and low-power memories and logic devices with infinite endurance.
The remainder of this review is organized as follows: Sec.II deals with the discovery of iPMA at magnetic metal/oxide interfaces and early studies of the phenomenon. Ab initio theoretical studies of the origin of this iPMA are covered in Sec. III. Section IV discusses the use of this iPMA in perpendicular STT-MRAM and the resulting scalability of these memories. Emerging research directions that take advantage of this phenomenon are dealt with in Sec.V, which covers the voltage control of the iPMA, and Sec. VI, where some other recent R&D topics taking advantage of this phenomenon are considered.
II. PMA AT MAGNETIC TRANSITION METAL/OXIDE INTERFACES: A HISTORICAL PERSPECTIVE
A. First observation with AlOx formed by rf oxidation and natural oxidation
iPMA at magnetic transition metal/oxide interfaces was first observed in 2002 in a study of the oxidation of an Al layer to form an alumina-based magnetic tunnel junction (Monso et al., 2002). Natural oxidation and plasma oxidation were both used and results were very similar. The samples investigated con-sisted of a Pt underlayer surmounted with Co0.6 nm=Al tAl.
Following oxidation, the out-of-plane magnetic hysteresis loop was measured based on the extraordinary Hall effect (EHE) (also called the anomalous Hall effect) with magnetic field applied perpendicular to the plane of the sample. The EHE is sensitive to the out-of-plane component of magnetization. Figure 1 illustrates the effects observed for a 1.5-nm-thick Al layer exposed to an oxygen plasma (5 × 10−2 mbar with a rf power of0.4 W=cm2). During oxidation, the oxygen penetrates inside the Al layer by diffusing along the grain boundaries, gradually gaining access to the inner part of the grains (Bae et al., 2002). Thus the Al is progressively transformed into amorphous alumina. After an adequate duration of exposure to the oxygen plasma, the Al layer becomes fully oxidized. If oxidation
continues beyond this point, the oxygen starts to penetrate the underlying magnetic electrode where it diffuses inside the Co layer through the grain boundaries, leading to overoxidation of the barrier. Figure 1 shows the magnetic response of the underlying magnetic electrode with various durations of expo-sure to the oxygen plasma, as meaexpo-sured by EHE. For short durations (less than 2 min, for example, 1 min 30 s), a slanted hysteresis loop is observed with zero remanence and a relatively large saturation field of about 5 kOe. In these conditions, the Co anisotropy is in plane despite the use of a Pt underlayer, indicating that the interfacial perpendicular anisotropy provided by the Pt layer is too weak in these experiments to overcome the easy-plane demagnetizing energy of the Co layer. With oxygen exposure lasting 2 min, a square hysteresis loop is observed, with 100% remanence and a low coercive field of about 20 Oe (see the inset in Fig. 1). These parameters indicate that the anisotropy of the Co layer has clearly changed and is now out of plane even though the amplitude of the EHE is the same as in the underoxidized sample, indicating that the Co layer is not yet oxidized. Since the oxygen penetrates from the upper surface, Monso et al. (2002)hypothesized that an interfacial anisotropy appeared at the Co=alumina interface as a result of the oxidation process. This hypothesis was later confirmed by XAS and XPS experiments. When the film is further oxidized, the square shape of the hysteresis loop, and thus the interfacial perpendicular anisotropy, is maintained up to 3 min of oxidation time, although a drop in the EHE amplitude is observed indicating that the Co starts to become oxidized, probably due to diffusion of the oxygen along the grain boundaries (Bae, Shin, and Lee, 2002). Finally, for oxidation durations exceeding 3 min, the hysteresis loop becomes slanted with a high saturation field indicating that perpendicular anisotropy is lost. The loss of perpendicular anisotropy is therefore associated with the disappearance of the Co=alumina interface and formation of a Co=CoO=alumina bottom electrode.
These effects were subsequently reproduced for various thicknesses of the Al capping layer (Rodmacq et al., 2003). The dramatic variation in out-of-plane susceptibility of the Co layer induced by the oxidation of Al into alumina and the FIG. 1. Out-of-plane hysteresis loops measured for Pt3 nm=Co 0.6 nm=Al 1.5 nm based on EHE after various durations of exposure to an oxygen plasma. FromRodmacq et al., 2003.
associated increase in Co=AlOx interfacial anisotropy can be clearly observed when the low-field slope of the EHE hysteresis loops is plotted against time (Fig.2). This repre-sentation reveals changes to the out-of-plane susceptibility of 3 orders of magnitude. The maximum out-of-plane suscep-tibility is associated with the optimal barrier oxidation con-ditions, corresponding to the situation where the oxygen atoms reach the Co=Al interface transforming it into a Co=alumina interface. Taking advantage of this correlation, it was proposed that the measurement of the out-of-plane susceptibility could be used to control and optimize the oxidation of tunnel barriers in MTJs (Monso et al., 2002), a technique which could be implemented in situ during growth using the magneto-optic Kerr effect (MOKE). If the thickness of the Al capping layer is varied, the optimum plasma oxidation time shifts toward longer times (Fig.2). This shift could be readily explained by considering that the thicker the barrier, the longer it will take for the oxygen to reach the underlying Co interface. In parallel to this increased penetra-tion time, the maximum in EHE slope becomes broader indicating that the oxidation process is less homogeneous as the Al thickness increases.
Similar trends were observed using natural oxidation of the Al layer and a CoFe bottom electrode instead of a Co one (Monso et al., 2002).
B. A general phenomenon at magnetic metal/oxide interface: Soon after, SPINTEC demonstrated that this phenomenon is quite common and can be observed with a large variety of amorphous or crystalline oxides which may be formed from the metallic element by natural oxidation or by plasma oxidation, or even when the oxide layer is directly rf sputtered from an oxide target. The phenomenon is therefore relatively robust. This iPMA is already present in as-deposited samples, but can be maximized by annealing the structure (see Sec. II.E). As an example, Fig. 3shows a similar crossover of anisotropy to that illustrated in Fig. 1, but for a CrOx
barrier. For this figure, the samples consisted of a Pt under-layer surmounted by Co0.6 nm=Cr tCr, and the EHE loops
were measured 12 h after deposition and exposure to air. For very thin Cr layers, full oxidization is achieved naturally by exposure to air, and the anisotropy is perpendicular. However, for thicker Cr layers, natural oxidation cannot fully oxidize the Cr down to the Co interface and therefore the perpendicular anisotropy disappears.
Figure 4 shows observations of the same maximum of out-of-plane susceptibility as illustrated in Fig. 2 for four different oxide materials formed by natural oxidation of the FIG. 2. Out-of-plane susceptibility of Pt3 nm=Co 0.6 nm=Al
tAl measured based on EHE as a function of the duration of
exposure to the oxygen plasma for various Al layer thicknesses. FromRodmacq et al., 2003.
FIG. 3. EHE hysteresis loops for a series of Cr-capped samples naturally oxidized by exposure to air, measured with a field
applied out of plane. Sample composition: Pt 3 nm=Co
0.6 nm=Cr tCr.
FIG. 4. Variation of the out-of-plane susceptibility for naturally
oxidized samples composed of Pt3 nm=Co 0.6 nm=MOx tM.
The samples were naturally oxidized by exposure to oxygen at a partial pressure of 160 mbars for 30 min. Samples were then capped by applying a protective Pt layer to avoid further oxidation due to air exposure. FromManchon et al., 2008.
corresponding metallic element. Interestingly, some of these oxides are amorphous (AlOx, TaOx), whereas others are polycrystalline (MgO, RuO). The optimum thickness of the metallic layer, allowing the maximum out-of-plane suscep-tibility to be reached, depends on the nature of the element. This effect can be explained in terms of the different kinetics of oxidation for the different oxides and the self-limiting oxidation which occurs with some oxides such as TaOx and AlOx.
C. Correlation between PMA and electron-specular reflection in specular spin valves
The key role played by the degree of oxidation along the magnetic metal/oxide interface was further demonstrated by experiments performed in 2003 which found a correlation between the amplitude of the iPMA at the Co=AlOx interface and the degree of specular reflection at the same interface when the trilayer was inserted into current-in-plane (CIP) specular spin valves (Rodmacq et al., 2003). This correlation was established by carrying out two experiments in parallel. The first experiment measured perpendicular anisotropy at the Co=AlOx interface in Pt 3 nm=Co 0.6 nm=Al 1.5 nm sand-wiches as a function of the duration of exposure to an oxygen plasma, as described before. The second experiment consisted of growing spin valves composed of Pt 3 nm=Co 3 nm=Ru 0.5 nm=Co 2 nm=Cu 3 nm=Co 1.5 nm=Al 1.5 nm (Dieny et al., 1991) and similarly measuring their CIP properties (resistance and GMR) as a function of the duration of exposure of the capping layer to the oxygen plasma. The same partial pressure of oxygen and rf power were used in the two experiments so that the two Al capping layers could be considered to be oxidized in identical conditions. In the second series of experiments, the gradual oxidation of Al to form AlOx changed the electron scattering pattern at the Co=AlOx interface from diffuse scattering when the interface is poorly or not oxidized to specular reflection when the metal/ oxide interface forms a perfect wall of energy for electron conduction. Oxygen vacancies present at the interface can be qualitatively viewed as holes in this wall, and they will generate electron diffusion. When no more vacancies remain, electrons will be perfectly reflected by this interface, allowing them to conserve their momentum parallel to the interface. In these conditions, a minimum in CIP resistance and a corre-sponding maximum in GMR amplitude are measured due to the decreased scattering at the Co=AlOx interface (Egelhoff et al., 1997;Veloso et al., 2000;Da Costa et al., 2002). If the Al layer is oxidized beyond the optimal conditions, CIP resistance increases due to the additional resistance introduced by the oxidation along the Co grain boundaries. This increased resistance is associated with a decrease in GMR amplitude due to additional scattering and the reduced specular reflection caused by the inhomogeneous oxygen penetration into the Co layer (Rodmacq et al., 2003).
The data obtained for these two sets of experiments are reported in Fig.5as a function of the duration of exposure to the oxygen plasma. Clearly, the maximum perpendicular anisotropy is measured in the same oxidation conditions where the maximum specular reflection is obtained at the Co=AlOx interface in specular spin valves. This maximum
specular reflection corresponds to the minimum CIP resis-tance and correlatively to the maximum CIP GMR. These correlations confirmed that the maximum iPMA is obtained when the oxygen ions have reached the Co=AlOx interface, when no more metallic Al remains along the interface. This corresponds to the point when the density of oxygen vacancies along the interface has been drastically reduced.
D. Physicochemical characterization (XAS, XPS) of the metal/ oxide interface and correlation with anisotropy
To get a deeper insight into the physicochemical properties of the magnetic metal/oxide interface, XAS and photoemission experiments were performed on a series of Pt=Co=MOx samples with M¼ Al, Mg, Ta, and Ru. The results of these experiments are described in Figs.6–8for a Co=AlOx interface (Manchon et al., 2008). The samples studied were composed of an underlayer (Pt 3 nm) surmounted by Co0.6 nm=Al 1.6 nm. Samples were not annealed, they were oxidized using an oxygen rf plasma at a partial pressure of3 × 10−3 mbar and an rf power of 10 W. Figure6shows the EHE response of these samples when an out-of-plane field was applied after various durations of exposure to the oxygen plasma. The observations are consistent with those shown in Fig.1.
Thus, for samples oxidized for durations shorter than 25 s, the magnetization loops show no hysteresis and nearly zero remanence, indicating that the magnetic anisotropy is in plane [Fig.6(b)]. With intermediate oxidation times, between 30 and 40 s, square hysteresis loops were observed with sharp magnetization reversal and nonzero coercivity associated with out-of-plane anisotropy. When the duration of oxidation exceeded 45 s, the hysteresis loops were once again slanted with zero remanence and large saturation fields. To quantify the FIG. 5. Experimental observation of the correlation between the maximum iPMA at the Co=AlOx interface in Pt=Co=AlOx and the maximum specular reflection in specular spin valves with a free Co=AlOx layer, as a function of the degree of oxidation of the capping layer (AlOx). These data confirm that the iPMA is maximized when the oxygen has reached the Co=AlOx interface producing a very sharp energy wall for the conduction electrons at the metal/oxide interface which is then characterized by a very small number of oxygen vacancies. FromRodmacq et al., 2003.
perpendicular anisotropy, the EHE was also measured with an in-plane field and the anisotropy field was derived from these measurements (Manchon et al., 2008); see Fig. 6(c). The maximum iPMA was observed with oxidation durations between 35 and 40 s, when the hysteresis loops in Fig.6(c) are the most square.
Interestingly, these measurements with in-plane field also revealed that the disappearance of the squareness of the
hysteresis loops after more than 45 s of oxidation is not immediately due to a loss of perpendicular anisotropy but to the fact that magnetization is split into up domains and down domains due to oxygen diffusing within the Co layer at the grain boundaries. This local Co oxidation disrupts the in-plane exchange stiffness and facilitates the formation of domain walls across the grain boundaries. In fact, the Co grains become almost uncoupled so that the magnetization can easily split into up domains and down domains to minimize the magnetostatic energy. This causes the hysteresis loop to become slanted.
Figures7and8show the XAS and XPS spectra obtained for the same series of samples. A direct correlation can therefore be established between the magnetic and physicochemical proper-ties. XAS measurements were performed around the Co L2;3 absorption edges (760–800 eV). Figure 7 shows the XAS spectra for Pt=Co=AlOx trilayers exposed to the oxygen plasma for different durations (hereafter called oxidation time for simplicity). XAS spectra for pure Co and CoO are shown as references in Figs.7(a) and 7(c), respectively. For t <25 s [Fig.7(a)], the spectra for the trilayer resemble those for pure Co. With30 < t < 40 s [Fig.7(b)], shoulders appear in the absorption spectra indicating the presence of small contribu-tions due to the formation of CoO. At45 < t < 60 s [Fig.7(c)] these shoulders become very clear and the absorption spectra strongly resemble that for pure CoO.
Figures7(d)–7(f)show the derivatives of the XAS spectra. These derivatives more clearly reveal the presence of CoO in the Co layer, and the vertical lines indicate the energy of the FIG. 6. (a) Sample geometry, (b) EHE vs out-of-plane field for
various durations of exposure to the oxygen plasma, and (c) anisotropy field vs oxidation time determined from EHE
measured while applying an in-plane field. From Manchon
et al., 2008.
FIG. 7. XAS spectra measured for Co L2;3 within Pt=Co=AlOx trilayers for (a) underoxidized, (b) optimally oxidized, and (c) overoxidized samples, and their corresponding derivatives (d), (e), and (f) at the Co L3edge. Reference spectra for pure Co are shown in (a) and (d) and for CoO in (c) and (f). The solid and dotted vertical lines indicate the energy positions of the shoulders in the XAS spectra due to the presence of Co and CoO. FromManchon et al., 2008.
peaks on the derivative corresponding to Co (solid line) and CoO (dashed line). For short oxidation times [Fig.7(d)] only peaks corresponding to pure Co are present. At intermediate oxidation times [Fig. 7(e)] a small peak appears at 777 eV, corresponding to a small proportion of CoO. Finally, for long oxidation times [Fig. 7(f)], two CoO peaks are present, although they remain smaller than the peaks detected with pure Co. These observations clearly indicate that no oxygen atoms are present in the Co layer after short oxidation times. Some oxidation, probably near the interface, appears at intermediate oxidation times. And finally, after considerable exposure, oxygen penetrates deeply into the Co layer.
To obtain further information on the chemical composi-tion of the Co layer, XPS measurements were performed setting the beam line energy to hν ¼ 1130 eV to probe Co 2p levels (Manchon et al., 2008); see Fig. 8. It should be remembered that XPS is surface sensitive, so that the spectra provide information on the chemical composition of the Co monolayer (ML) which is directly in contact with the AlOx layer.
Figure 8shows the Co 2p spectra obtained for the same series of samples as in Figs. 6and7. The spectrum for the t¼ 60 s sample is very similar to that obtained for pure CoO (Grimbolt, Bonnelle, and Beaufils, 1976;Carson, Nassir, and Langell, 1996). The two main peaks (lying at 796.3 and 781.1 eV) correspond to CoO 2p1=2 and CoO 2p3=2 core levels, respectively, while the two satellite peaks (denoted S, with positions at 803.3 and 786.7 eV) are produced by the charge transfer between O 2p and Co 3d, respectively (Grimbolt, Bonnelle, and Beaufils, 1976; Carson, Nassir, and Langell, 1996). The spectrum for the t¼ 15 s sample is similar to that of pure cobalt (Sicot et al., 2005) with Co 2p1=2and Co2p3=2detected at binding energies of 792.5 and
778.1 eV, respectively. This spectrum clearly shows that Co is completely unoxidized at t¼ 15 s. At t ¼ 20 and 25 s, a small contribution of Co-O bonds appears. Between t¼ 30 and 40 s, both Co-O and Co-Co bonds coexist, while for oxidation
times exceeding 45 s, the Co contribution has completely disappeared.
These XPS spectra therefore clearly show that the compo-sition at the Co=AlOx interface changes from quasipure Co to CoO during oxidation and that the maximum iPMA is obtained in conditions where Co-O bonds have formed across the Co=AlOx interface, but where the topmost interfacial Co layer is not yet oxidized. In these conditions, in the Co monolayer in contact with the AlOx oxide layer, Co-Co bonds still prevail, whereas Co-O bonds prevail across the interface. These observations, together with the fact that the maxi-mum iPMA correlates with the maximaxi-mum specular reflection, indicate that iPMA arises from the hybridization effect that occurs across the Co-oxide interface between the Co orbitals (particularly out-of-plane orbitals dxz, dyz, and dz2) and the sp
O orbitals. This hybridization eliminates the degeneracy between the magnetic transition metal 3d orbitals pointing out of plane and those with planar symmetry (dxy and dx2−y2)
giving rise in a first approximation to a crystalline field Δc¼ Eðyz; zx; z2Þ − Eðxy; x2− y2Þ: ð9Þ
This crystalline field can yield a relatively large surface or interfacial anisotropy even in materials where spin-orbit coupling is relatively weak (Bruno, 1989). The amplitude of the perpendicular anisotropy correlates with the anisotropy in the magnetic transition metal orbital momentum; the PMA energy can be expressed as
ΔEPMA¼ G H ξ 4μBðm ⊥ orb− m == orbÞ; ð10Þ
where m⊥ð==Þorb is the out-of-plane (respectively, in-plane)
orbital moment, ξ is the spin-orbit-coupling parameter, and G=H are band-structure-dependent coefficients (Bruno, 1989; Manchon et al., 2008). Note that Bruno’s model is approxi-mate and valid only with large exchange splitting and when off-site and/or spin-mixing spin-orbit-coupling are negligible (van der Laan, 1998;Andersson et al., 2007;Li et al., 2013). However, it can still be used to qualitatively determine the magnetic anisotropy arising from the coupling between the anisotropy of the 3d orbital moment ⃗l and the magnetic moment ⃗s of the magnetic atoms through the spin-orbit coupling ξ⋅⃗l⋅⃗s. This interpretation of the origin of the iPMA at interfaces between transition magnetic metals (Co, Fe, CoFeB) and oxides (AlOx, MgO, HfOx, CrOx, TaOx) was later confirmed by ab initio calculations (Nakamura et al., 2010; Shimabukuro et al., 2010; Yang et al., 2011; Liang et al., 2014; see Sec.III).
X-ray magnetic circular dichroism (XMCD) experiments performed on MgO=CoFeB interfaces (Tsai et al., 2012) and on Fe=MgO interfaces (Okabayashi et al., 2014) also con-firmed this interpretation. As with the Co=AlOx samples described, Okabayashi et al. observed the existence of extra prepeaks in the XAS spectra for the O K edge. These supplementary peaks clearly indicate that Fe-O bonding occurs at the MgO=CoFeB (Fe=MgO) interfaces, leading to the hybridization of Fe and O orbitals. Furthermore, the strength of the PMA in annealed samples correlated with FIG. 8. Co 2p XPS spectra for Pt 3 nm=Co, 0.6 nm=Al,
1.6 nm þ rf-plasma oxidation for various oxidation times. Right: illustration of how the oxygen atoms penetrate the structure as the oxidation time increases. FromManchon et al., 2008.
the orbital hybridization of Fe-3d and O-2p orbitals, as assessed using the Fe orbital moment determined from XMCD measurements.
E. Influence of annealing
The influence of annealing on iPMA at magnetic transition metal/oxide interfaces was thoroughly studied for the first time in 2009 (Rodmacq et al., 2009). In their work, Rodmacq et al. studied a series of samples composed of Pt3 nm=Co, 0.6 nm=Al 1.6 nm after rf-plasma oxidization of the Al layer for various oxidation times covering the whole range from underoxidized to overoxidized. The samples were sub-sequently annealed at various temperatures up to 450 °C. To conveniently represent the data obtained, the magnetization reversal nucleation field was determined from the Hall hysteresis loops. This nucleation field (Hnuc) is the
character-istic field at which the magnetization is no longer saturated and starts to switch directions. When a decrease from positive saturation occurs, the nucleation field will be positive for samples with in-plane magnetization (0% remanence) and negative for samples with out-of-plane magnetization (∼100% remanent magnetization). To conveniently describe the var-iations of Hnucover several orders of magnitude, the following
notation was introduced: H¼ logðjHnucjÞ, where H will
have the same sign as Hnuc, i.e., negative for out-of-plane
magnetized samples and positive for in-plane magnetized samples. Figure 9(a)shows a color-coded illustration of H
plotted as a function of annealing temperature (100 °C to 450 °C) and oxidation time (oxidation by exposure of the 1.6-nm Al capping layer to an rf oxygen plasma with exposure times between 15 and 60 s). At low annealing temperatures, similar results to those described for annealed samples are obtained. An optimum oxidation time of around 35 to 40 s is observed, where the nucleation field is maximized along with the iPMA, as previously explained. In as-deposited or weakly annealed samples, the range of oxidation times over which iPMA is observed is relatively narrow [dark (blue) zone in Fig. 9(a)]. However, it is interesting to note that upon annealing this region broadens, suggesting that the oxygen migrates to the Co=AlOx interface to allow its perfect oxidization and the formation of Co-O-Al bonds all over the interface.
This hypothesis was upheld by three other observations: (i) Fig. 9(b) (Manchon et al., 2008) shows the ratio of Al ions bonded to oxygen normalized for the total number of Al ions in the AlOx layer, as measured by XAS. This ratio is plotted against the initial oxidation time. Since XAS is sensitive to the bulk of the layer, the data clearly indicate that some of the oxygen has disappeared from the bulk of the layer following annealing at 350 °C. (ii) In parallel, XPS data (Manchon et al., 2008) indicate that annealing increases the number of interfacial Co atoms bound to O. (iii) The Hall angle reaches a maximum value in the region corresponding to high annealing temperatures and low to moderate oxidation times [not shown, Fig. 4 in
FIG. 9. (a) H (see text) (color code) plotted as a function of annealing temperature (TA) and initial oxidation time for samples
composed of Pt3 nm=Co, 0.6 nm=Al, 1.6 nm oxidized by rf oxygen plasma. (b) Ratio of Al ions bonded to oxygen in the plasma-oxidized AlOx layer, as measured by XAS, vs oxidation time in as-deposited and annealed samples (350 °C). FromManchon et al., 2008. (c) Ratio of Co ions bonded to oxygen at the Co=AlOx interface, as measured by XPS, vs initial oxidation time in as-deposited and annealed samples. FromManchon et al., 2008.
Rodmacq et al. (2009)]. These observations can be explained if oxygen from the inner part of the AlOx layer or from the Co grain boundaries (for overoxidized samples) migrates toward the Co=AlOx interface upon annealing, suggesting that this interface is the most stable location for oxygen ions. Note that similar results were obtained when MgO layers were substituted for AlOx layers (Manchon et al., 2008; Rodmacq et al., 2009).
The effective anisotropy field in samples with out-of-plane magnetization as well as the iPMA energy were extracted by measuring the EHE loops while applying an in-plane field to a series of plasma-oxidized samples composed of Pt 3 nm=Co, tCo=Al 1.6 nm after oxidation times ranging from
15 to 60 s and annealed at various temperatures between 100 °C and 450 °C. The thickness of the Co layer varied between 0.5 and 3.8 nm. Figure10(a) shows the anisotropy field (Han) plotted as a function of annealing temperature and
oxidation time for the series of samples with tCo¼ 0.6 nm.
The color scale is in kOe. Maximal PMA is clearly obtained at around 35 s oxidation time after300 °C annealing. In that region of the graph, superconducting quantum interference device (SQUID) measurements gave a value of103 emu=cm3 for the saturation magnetization of the Co layer. This value corresponds to an effective anisotropy constant
Keff ¼ MsHan=2 of 0.8 MJ=m3 (8 × 106 erg=cm3), which
is larger than in most Pt- or Pd-based magnetic multilayers (Ikeda et al., 2005, 2008). In these oxidation and annealing conditions, the Co=AlOx interface is optimally oxidized. As previously discussed, annealing promotes homogeneous oxi-dation along the interface, decreases roughness at the inter-face, modifies the Pt=Co interinter-face, and thus allows the sum of the two interfacial anisotropies at Pt=Co and Co=AlOx to largely overcome the demagnetizing energy. The underox-idation of the samples treated for oxunderox-idation times shorter than 25 s does not allow maximal PMA to be attained as the number of oxygen atoms at the Co=AlOx interface is insufficient.
To extract the sum of the interfacial anisotropies at the Pt=Co and Co=AlOx interfaces, KefftCo was plotted against
tCo in Fig.10(b)for as-deposited and annealed samples. The
slope of the linear part of these curves gives the effective bulk anisotropy which, here, is essentially the demagnetizing energy of the Co layer (−μ0Ms2=2). The intercept with the y axis gives the sum of the interfacial anisotropy at the Pt=Co and Co=AlOx interfaces. Thus, after annealing at325 °C for 30 min, an interfacial anisotropy of KPt=Cos þ K
2.8 mJ=m2 (1 mJ=m2¼ 1 erg=cm2) is measured. Since the
interfacial anisotropy at the Pt=Co interface was previously reported to be in the range0.6–1.4 mJ=m2(Guoa et al., 2006; Yakushiji et al., 2010), this result implies that the iPMA at the Co=AlOx interface is in the range of1.4–2.2 mJ=m2, i.e., it is as large or even larger than that at the Pt=Co interface.
A similar order of magnitude was obtained at CoFe=MgO interfaces (Nistor et al., 2010). This order of magnitude was subsequently confirmed by various groups (Ma et al., 2012; Koo et al., 2013; Lambert et al., 2013) and by ab initio calculations (Niranjan et al., 2010; Yang et al., 2011). This result is remarkable considering how weak the spin orbit is in Co and AlOx. Indeed, a Pt=Co interface is commonly considered to be the archetype of high interfacial anisotropy, and this property is assumed to rely on large spin-orbit coupling. Other interfaces such as Co=Ni (Johnson et al., 1996;Gottwald et al., 2012) or Cu=Ni (Johnson et al., 1996) do exhibit perpendicular interfacial anisotropy with weak spin orbits, but their interfacial anisotropy is twofold to threefold weaker than that measured at CoFe=oxide or (Pt=Co) interfaces.
F. Correlation between PMA and tunnel magnetoresistance in MgO-based MTJ
A study carried out early in 2010 established a correlation between the amplitude of the interfacial PMA at CoFe=MgO interfaces and the corresponding TMR in MTJ, where the tunnel barrier was prepared by applying natural oxidation conditions (Nistor et al., 2010). The structures used to investigate how anisotropy varied with Mg thickness were SiO2=Ta 3=Pt 30=Co70Fe30 1=Mg tMg=Ru 5 nm. The Mg
layer was naturally oxidized to form MgO by exposing the metallic Mg layer to oxygen at a pressure of 1 mbar for 450 s. The structures used to investigate the TMR amplitude were in-plane magnetized MTJ stacks of composition: Ta 3=CuN 60=Ta 5=PtMn 20=Co70Fe30 2=Ru 0.74=CoFeB 2=Mg FIG. 10. (a) Anisotropy field map (in kOe) for Pt 3 nm=Co,
0.6 nm=Al 1.6 nm samples, plasma oxidized for between 15 and 60 s and annealed at temperatures ranging from100 °C to 450 °C. (b) Interfacial anisotropy in naturally oxidized samples composed
of (thickness in nm) SiO, 2=Ta, 3=Pt, 20=Co, tCo=Al,
0.5==Nat:Ox:=Cu, 2=Pt 2, ð1 erg=cm2¼ 1 mJ=m2Þ. From
tMg=CoFeB3=Ta 10. The Mg layer was oxidized under the
same conditions as those used for the first series of samples. Both series of samples were annealed at ∼330 °C in 10−6 mbar vacuum for 1 h prior to characterization.
Figure11(a)shows the anisotropy fields for the out-of-plane magnetized first series of samples (Pt=CoFe==Mg=natural oxidation based) alongside the TMR for the second series of samples, as measured by the CIP-TMR technique (Worledge and Trouilloud, 2003). The results of the two measurements clearly correlate, and the same Mg thickness produces maximal perpendicular anisotropy for the first series of samples and the maximum TMR in the second series. Since the samples were naturally oxidized, this means that these two maxima occur for the same degree of oxidation of the CoFe=MgO interface. This observation implies that the same mechanism, i.e., the formation of CoFe-O bonds at the
interface during oxidation, influences both the TMR ampli-tude and the interfacial anisotropy. This is consistent with the origin of the iPMA at magnetic transition metal/oxide inter-faces in terms of hybridization between O p and Co(Fe) dz2
orbitals, as discussed, and also with the easier penetration of Δ1electrons through the MgO barrier when it is O terminated
(Butler et al., 2001)
A similar comparison was performed using CoFeB in place of CoFe [Fig.11(b)] (Nistor et al., 2010). The main result of this comparison is that in Pt=CoFeB1.1 nm=MgO magneti-zation lies in the plane of the film, whereas in Pt=CoFe 1 nm=MgO a strong out-of-plane anisotropy is observed. These experiments therefore demonstrated that the presence of B at the CoFeðBÞ=MgO interface considerably reduces the iPMA. The presence of boron prevents hybridization between the Co(Fe) orbitals and the oxygen sp orbitals. The B is not absorbed away from the MgO interface upon annealing because in this experiment, the buffer layer (Pt) is a noble metal (You et al., 2008;Mukherjee et al., 2009). Therefore the B remains in the CoFeB layer right next to the CoFeB=MgO interface where it hampers PMA. Comparing the results presented in Figs. 11(a) and 11(b) shows how important it is to attract the B away from the MgO interface in CoFeB=MgO-based MTJ upon annealing so as to benefit from the interfacial PMA at the CoFe=MgO interface while also maximizing the TMR amplitude (Nistor et al., 2010).Oh et al. (2014) subsequently confirmed this conclusion by comparing levels of iPMA in CoFeB=MgO for structures associated with various underlayers including Ta and Hf (which attract B and therefore produce large PMA) and Pt and Pd (which are not good B getters and therefore do not promote interfacial PMA).
G. First observations of PMA at Ta=CoFeB=MgO interfaces The next important step toward the use of this interfacial PMA in out-of-plane MTJ was achieved by Ikeda et al. (2010) at Tohoku University when they investigated out-of-plane mag-netized Ta=CoFeB=MgO-based MTJs. From a basic research point of view, this is a specific case of the various systems in which PMA was observed at transition metal/oxide interfaces since 2002. However, from a technical point of view, the results obtained by Ikeda et al. are quite important since they demon-strated that a large TMR and a large PMA with a relatively low STT switching current could be obtained in the same MTJ stacks. The idea for this study was as follows. The experiments byNistor et al. (2010)pointed out the importance of attracting the B away from the CoFeB=MgO interface to induce a strong PMA at this interface. Ikeda et al. did this by substituting a Ta underlayer for the Pt underlayer used by Nistor et al. Ta is known to be a good B getter, i.e., it is capable of drawing the B out from the initially amorphous CoFeB layer during postdeposition annealing of the MTJ (Yuasa and Djayaprawira, 2007; Kozina et al., 2010). Figure12shows the stacks used as well as some of the main results obtained. The MTJs investigated were composed of underlayer=Ta 5=Co20Fe60B20 ðtCoFeB from
1.0 to 1.3 nmÞ=MgO ðtMgO 0.85 or 0.9 nmÞ=Co20Fe60B20
ðfrom 1.0 to 1.7 nmÞ=Ta 5=Ru 5 (all thicknesses in nano-meters) [Fig. 12(a)]. Electron-beam lithography and Ar-ion milling were used to produce circular sample devices FIG. 11. (a) Variation in the TMR ratio in planar CoFeB-based
MTJ and in the perpendicular anisotropy of a Pt=CoFe=MgO bottom electrode as a function of the thickness of the naturally oxidized Mg barrier. The MgO layers were prepared by natural oxidation in the same conditions for the two sample series. (b) Comparison of TMR in in-plane-magnetized CoFeB-based
MTJ and of the anisotropy in Pt=CoFeB1.1 nm=MgO bottom
electrode for various Mg thicknesses. The bottom electrode contains B which the Pt buffer layer prevents from moving away from the MgO interface upon annealing. The presence of B along the CoFeB=MgO interface inhibits the interfacial perpendicular anisotropy at CoFeB=MgO so that the magnetization of the CoFeB layer remains in plane. The coercive field is plotted alongside the TMR amplitude; no correlation exists in this case. FromNistor et al., 2010.
measuring 40 or 150 nm in diameter [Fig.12(b)]. Figure12(c) shows that after annealing at350 °C a TMR of up to 120% was obtained. This increase in TMR amplitude between the as-deposited state and after optimal annealing (here 350 °C) is due to the improved crystallinity of the bcc MgO barrier and to the recrystallization of the CoFeB electrodes into bcc CoFe as the B is absorbed into the Ta buffer and capping layers. This improvement in the crystallinity of the magnetic electrodes and of the tunnel barrier yields the spin-filtering mechanism
through which the giant tunnel magnetoresistance of crystal-line MgO-based MTJs is generated (Butler et al., 2001;Parkin et al., 2004; Yuasa et al., 2004; Yuasa and Djayaprawira, 2007). The degradation of the TMR observed above350 °C is ascribed to diffusion of the Ta through the CoFeB layers toward the MgO barrier (Ikeda et al., 2008).
In these samples, thanks to the strong interfacial anisotropy at the CoFeðBÞ=MgO interface, the magnetization of the CoFeB is pulled out of plane only when the CoFeB layers are thin enough to allow the iPMA to overcome the easy-plane demagnetizing energy. In this study, samples with CoFeB thicknesses of less than 1.3 nm could be magnetized out of plane after annealing at300 °C.
Figure 12(d) shows typical hysteresis loops obtained in STT switching experiments. Switching occurs at relatively low current densities of aroundð2–4Þ × 106 A=cm2, indicat-ing that the Gilbert dampindicat-ing in these systems is relatively weak compared to that measured for Co=Pt-based multilayers. Indeed, in STT experiments, the critical current for switching is proportional to the Gilbert damping (Slonczewski, 1996; Sun, 2000; see Sec. IV for further details). In out-of-plane magnetized samples, the critical current for switching in the macrospin model was determined (Sun, 2000) and is given by
Iperpc ¼ 4e ℏ αk BT gp Δ; ð11Þ
where α is the Gilbert damping constant, e is the electron charge,ℏ is the Planck constant, kBis the Boltzmann constant,
T is the temperature, p is the spin polarization, Δ is the thermal stability factor¼ ΔE=kBT¼ KeffV=kBT, and g is a
function of the spin polarization of the tunnel current and of the angle between the magnetizations of the free and reference layers (Berger, 1996,1999;Slonczewski, 1996,1999).
The Gilbert damping constant α was measured by ferro-magnetic resonance (FMR) experiments [Fig. 12(e)] and found to significantly increase at low CoFeB thicknesses, in particular, within the range where perpendicular anisotropy is observed (below 1.3 nm). This phenomenon is associated with diffusion of Ta into the CoFeB layer, reduction in the ordering temperature of the CoFeB layer as it thins, and with a spin-pumping effect (Kato et al., 2012;Shaw, Nembach, and Silva, 2012). In terms of STT-MRAM applications (see Sec.IV), this increase in damping at low thicknesses means the critical current for STT switching will increase. This increase is a drawback, but it can be limited or even avoided through material optimization, as seen in Sec.IV.
The thermal stability factor Δ was determined from the variations in the critical current for switching versus write current pulse duration [Fig.12(f)] in the thermally activated regime (for current pulses longer than∼10 ns) using
Ic¼ Ic0 1 −kBT ΔEln τ τ0 ð12Þ (Koch, Katine, and Sun, 2004; Li and Zhang, 2004). A thermal stability factor of 43 was obtained for a 40 nm diameter MTJ, which corresponds to a retention time of ∼140 yr for a single MTJ cell. A thermal stability factor above
FIG. 12. Ta=CoFeB=MgO-based out-of-plane magnetized
MTJ. (a) Schematic representation of an MTJ device used to study TMR and spin-transfer-torque switching. (b) Top view of an MTJ pillar by scanning electron microscopy. (c) TMR amplitude plotted against annealing temperature. (d) Example of spin-transfer-torque switching experiments performed with current pulse widths of 1.0 s and 300 μs. (e) Variation of the Gilbert damping coefficient as a function of CoFeB thickness, determined from ferromagnetic resonance (FMR) experiments. (f) Critical current density for STT switching as a function of lnðτP=τ0Þ, τP¼ pulse width, τ0¼ attempt time ∼1 ns, from
70 is required for a 1-Gbit chip and a probability of one failure over time of 10−4.
At about the same period as Ikeda et al. made their observations, Worledge (2010) and Worledge et al. (2011, 2014) from IBM also observed a strong perpendicular anisotropy of interfacial origin in Ta=CoFeB=MgO-based MTJs. Worledge et al. investigated the influence of various buffer layers (Cr, Ta, Ru, V, Ti, Al, Mg, Ru, W) on the perpendicular anisotropy of buffer=Co60Fe20B20 t=MgO 0.9 nm=Fe 0.3 nm=5 TaN in samples with t ranging from 0.3 to 1.6 nm. The samples were annealed for 1 h at240 °C. Results indicated that the perpendicular anisotropy of the CoFeB layer was particularly strong with a Ta buffer layer. Thus, with Ta=CoFeB=MgO, an overall interfacial anisotropy of 1.8 mJ=m2 (1.8 erg=cm2) was observed, whereas with Ru=CoFeB=MgO, anisotropy was only 0.5 mJ=m2. This difference is mainly due to better absorption of the B away from the MgO interface upon annealing when a Ta underlayer is present. Significant intermixing between Ta and CoFeB was also observed in these experiments, which is much less pronounced between Ru and CoFeB.
All these results on Ta=CoFeB=MgO-based MTJ were extremely encouraging for the development of out-of-plane magnetized STT-MRAM and numerous studies subsequently emerged describing developments of STT-MRAM cells attempting to achieve long enough retention and sufficiently low switching current.
H. Interfacial PMA in epitaxial Fe=MgO-based systems iPMA at epitaxial Fe=MgO interfaces has been investigated by several groups (Lee et al., 2011;Koo et al., 2013;Lambert et al., 2013;Koziol-Rachwal et al., 2014). Examining the sign and amplitude of the effective anisotropy by magnetometry and FMR experiments,Lambert et al. (2013)showed that Fe-MgO interfaces possess a strong iPMA of1.0 0.1 mJ=m2in fully epitaxial heterostructures composed of MgO (100) substrate=V, 10 nm=Fe=MgO, 1.2 nm (001) or MgO (100) substrate=Cr,10 nm=Fe=MgO, 1.2 nm (001). As in sputtered samples, reorientation of the anisotropy from in plane to out of plane was observed below a certain critical thickness of the Fe MLs (6 nm for V=Fe=MgO and 4 nm for Cr=Fe=MgO). Magnetometry experiments revealed the presence of 2-nm magnetic dead layers in Fe MLs on V that do not exist on Cr. For a given Fe thickness, the demagnetizing energy is thus smaller in V=Fe=MgO than in Cr=Fe=MgO. When this difference is taken into account, the interfacial anisotropy at the Fe=MgO interface is found to be the same in the two series of samples (∼1 mJ=m2). Similar magnetic dead layers were reported by various groups at sputtered Ta=CoFeB interfaces (Ikeda et al., 2010; Worledge et al., 2011; Cuchet et al., 2014). This measured interfacial PMA was weaker than that measured by Koo et al. (2013) in Cr=Fe=MgO after annealing at 400 °C: Ks∼ 2 mJ=m2.Koo
et al. (2013)observed a strong increase in the interfacial PMA occurring between the 350 °C anneal and the 400 °C anneal that they ascribed to a variation of the interface composition due to oxygen atoms floating up from the Cr buffer layer and reaching the MgO interface. This hypothesis is consistent with
earlier experiments from SPINTEC (Monso et al., 2002; Rodmacq et al., 2003, 2009; Manchon et al., 2008) which demonstrated that the PMA reaches a maximum in conditions where the CoðFeÞ=MO interface is optimally oxidized (MO¼ oxide layer, i.e., MgO) so as to allow the formation of Co(Fe)-O-M interfacial bonds.
Koziol-Rachwal et al. (2014)also demonstrated that PMA could be obtained in (Fe=MgO) multilayers with large numbers of repeats on the condition that the Fe layers are thin enough to allow the interfacial PMA at Fe=MgO interfaces to overcome the demagnetizing energy. In Koziol-Rachwal et al. (2014)samples were epitaxially grown on an MgO (001) substrate and characterized by conversion electron Mössbauer spectroscopy (CEMS) and MOKE. In specific multilayers, ðFe 4ML=MgO 3MLÞN, PMA was
observed with an increased amplitude when the number of repeats N was varied from 10 to 20. The CEMS measurements with 57 Fe ML probes located at different sublayers revealed that the PMA was produced in the inner part of the multi-layered stack, whereas in the outer parts (top and bottom of the stacks), the magnetization was mostly in plane. Correlations between MOKE and CEMS experiments suggested a complex vortexlike magnetization distribution in the cross section of the stack. This was confirmed by micromagnetic simulations. Ding and Poon (2012) also observed PMA in epitaxially grown sandwiches composed of substrate MgOð001Þ= Co20Fe50Ge30=MgO 5 nm. The samples were grown by sputtering and annealed at 250 °C for 2 h. Ding and Poon (2012)introduced Ge into the CoFe so as to obtain a Heusler B2 phase characterized by high spin polarization and signifi-cantly lower damping than in CoFeB, as low as 0.0025 in bulk form (H. Lee et al., 2009;Wang et al., 2009); see Fig.12(e). In these experiments, the magnetization of the CoFeGe layer was observed to point out of plane for CoFeGe thickness tCoFeGe
below 1.3 nm. The PMA was mainly interfacial in origin, and an iPMA of∼0.9 mJ=m2was determined by extrapolation of the linear variation of KefftCoFeGevs tCoFeGeto zero thickness.
Similar findings have been reported for Heulser alloy based Ta=Co2FeAl=MgO multilayers (Gabor et al., 2013). I. Gilbert damping measurements in CoFeB=MgO-based MTJ
The Gilbert damping in Ta=CoFeB=MgO-based MTJ is a determinant parameter in spin-transfer-torque magnetization switching and has been studied by various groups (Ikeda et al., 2010;Liu et al., 2011;Devolder, Ducrot et al., 2013;Iihama et al., 2014).
Devolder et al. measured the anisotropy, the Landé g factor, and the Gilbert damping of series of Ta=CoxFe80−xB20
1 nm=MgO ultrathin films displaying PMA. They varied the CoFeB composition and annealing conditions. Measurements were performed by applying a vector network analyzer ferromagnetic resonance technique (Devolder, Barisic et al., 2013). Their results showed that, in Fe-rich FeCoB alloys, the PMA increases quite significantly upon crystallization, whereas the dampingα only increases slightly [e.g., in amorphous-Co20Fe60B20 1 nm, α ¼ 0.014 0.002, μ0ðHK− MsÞ ¼ 45 10 mT; in crystalline-Co20Fe60B20
1 nm, α ¼ 0.015 0.002, μ0ðHK−MsÞ ¼ 430 10 mT].